Is
NoTENSION DESIGN OF CONCRETE OR ROCK STRUCTURES ALWAYS
SAFE?FRACTURE ANALYSIS
By Zdenek P. Bazant,l Fellow, ASCE
ABSTRACT:
Plain concrete structures such as dams or retaining walls, as well as rock structures such as tunnels,
caverns, excavations, and rock slopes, have commonly been designed by elasticperfectly plastic analysis in
which the tensile yield strength of the material is taken as zero. The paper analyzes the safety of this "no
tension" design in the light of the finiteness of the tensile strength of concrete or the tensile strength of rock
between the joints. Through examples, it is demonstrated that: (1) the calculated length of cracks or cracking
zones can correspond to an unstable state; (2) the uncracked ligament of the cross section, available for
resisting horizontal shear loads, can be predicted much too large, compared to the fracture mechanics pre
diction; (3) the calculated loaddeflection diagram can lie lower than that obtained by fracture mechanics; (4)
the notension load capacity for a combination of crack face pressure and loads remote from the crack front,
calculated by elastic analysis on the basis of allowable compressive stress, can be higher than that obtained
by fracture mechanics; and (5) an increase in the tensile strength of the material can cause the load capacity
of the structure to decrease. Due to the size effect, these facts are true not only for zero fracture toughness
(notoughness design) but also for finite fracture toughness provided that the structure size is large enough.
Several previous studies on the safety of notension design, including the finiteelement analysis of a gravity
dam, are also reviewed.
It
is concluded that if the notension limit design is used, the safety factors of concrete
or rock structures cannot be guaranteed to have the specified values. Fracture mechanics is required for that.
INTRODUCTION
Concrete, and especially dam concrete, is a material of a
relatively low and highly variable tensile strength. The same
is true in the macroscopic sense of rock masses intersected
by a system of joints or preexisting cracks. Like rock joints,
construction joints may also have no tensile strength. There
fore, the design of unreinforced concrete structures such as
dams or retaining walls, as well as rock structures such as
tunnels, caverns, excavations, and rock slopes, has commonly
been made under the hypothesis that the material has no
tensile strength. Accordingly, in the simplified design of the
horizontal cross section of a dam, the distribution of the ver
tical normal stress has normally been assumed to be triangular
within the compressed part of the cross section (WES 1983;
BuRec 1987; Jansen 1988).
The "notension" design has traditionally been used for
masonryfor example stone arches, domes, or pillars. In
that case, the hypothesis of no tension is often nearly exactly
true, because of negligible strength and the dense spacing of
the joints. During the 1960s, the notension hypothesis was
introduced into finiteelement analysis [see, e.g., Zienkiewicz
(1971)]. In that case, the notension hypothesis is properly
implemented as the limit case of plasticity in which the tensile
yield strength approaches zero. Various yield criteria can be
used, for example, the Rankine criterion or MohrCoulomb
criterion [see, e.g., Owen and Hinton (1980)]. In the theory
of plasticity, it is proven [e.g., Hodge (1959)] that if yield
surface
A
lies within yield surface
B,
the limit load for surface
B
cannot be lower than the limit load for surface
A.
Thus,
for plastic materials, the notension design is guaranteed to
be on the safe side. Not so, however, for brittle materials.
The failure of brittle materials such as concrete or rock is
properly described by fracture mechanics rather than plastic
ity. Such materials do not fail simultaneously along the entire
'Walter P. Murphy Prof. of Civ. Engrg. and Mat. Sci., Northwestern
Univ., Evanston, IL 60208.
Note. Associate Editor: Steven
L.
McCabe. Discussion open until
June 1, 1996. To extend the closing date one month, a written request
must be filed with the ASCE Manager of Journals. The manuscript for
this paper was submitted for review and possible publication on June 6,
1994. This paper is part of the
Journal of Structural Engineering,
Vol.
122, No. I, January, 1996. ©ASCE, ISSN 07339445/96/000100020010/
$4.00
+
$.50 per page. Paper No. 8597.
2/ JOURNAL OF STRUCTURAL ENGINEERING / JANUARY 1996
failure surface, as required for applicability of the plastic limit
analysis. Rather, the failure propagates. Although the initi
ation of fracture is still governed by tensile strength, dams or
tunnels cannot be designed to fail at the initiation of fracture.
They must be designed so as to fail only after a large stable
crack growth. Instead of tensile strength, the failure is then
governed by the condition that the rate at which the potential
energy of the structureload system is released during fracture
propagation become equal to the energy per unit crack area
that the material can absorb. This is called the fracture en
ergy,
C
t
,
and represents the most fundamental failure char
acteristic of the material. In this regard, an important point
is that a structure of a higher tensile strength can store more
energy and can thus release stored energy during fracture
propagation at a higher rate (Bazant 1990). One must, there
fore, suspect that an increase of tensile strength could, at
least in some cases, reduce the load capacity of the structure
(Bazant 1990). In other words, the notension design might
not always guarantee safety if the material is brittle.
The question of safety of the notension design was raised
at the dam fracture workshop in Locarno, Switzerland (Dun
gar et al. 1990), and was intensely debated at the subsequent
dam fracture conferences in Boulder, Colorado (Saouma et
al. 1991) and Chambery, France (Bourdarot et al. 1994). By
simple examples of analytical solutions of rectangular speci
mens, it was shown (Bazant 1990) that, according to fracture
mechanics, tensile stresses can occur in notension plastic de
signs. Furthermore, the wellknown size effect of linear elastic
fracture mechanics (Bazant 1984; He et al. 1992) was shown
to imply that the notension design is not guaranteed to be
safe. In a subsequent study (Gioia et al. 1992), a typical
gravity dam with a large crack was considered to be over
topped and loaded by gravity, along with water pressure on
the upstream face and on the crack faces. Finiteelement anal
ysis showed that the loaddeflection diagram obtained by frac
ture mechanics with a finite fracture toughness can lie below
(in fact, significantly below) that obtained by notension plas
ticity.
The objective of this paper is twofold: (1) To present sev
eral new examples, which are easier to analyze and explain
than those presented earlier; (2) to review and interpret the
existing finiteelement results on the safety of the notension
design.
The notension hypothesis has, for a long time, been used
for reinforcedconcrete beams, columns, slabs, and other
structures. The reinforcedconcrete structures, however, are
not of concern here. For them, the safety of the notension
hypothesis is not disputed, because: (1) The contribution of
the tensile capacity of concrete to the load capacity of the
structure is small, compared to the contribution of the tensile
capacity of steel reinforcement; (2) the reinforcement forces
the tensile cracks to be densely distributed, i.e., prevents
them from localizing into wide, isolated cracks; and (3) the
yielding of steel reinforcement endows the loaddeflection
diagram of the structure with sufficient ductility, manifested
by a prolonged horizontal yield plateau. The yield plateau
implies the cause of failure to be a singledegreeoffreedom
plastic collapse mechanism rather than localization of damage
and propagation of fracture.
EXAMPLE 1: APPLIED FORCE REMOTE FROM CRACK
FRONT
To clarify the potential fallacy of the notension design, it
is helpful to consider simple specimens for which the solutions
according to linear elastic fracture mechanics (LEFM) are
available in handbooks such as those by Tada et al. (1985)
or Murakami (1987). Let us consider the rectangular concrete
specimen in Fig. l(a).
It
contains a horizontal crack of length
a
=
DI2
and has a unit thickness, width
D,
and height
H.
It
(e)
is loaded by the axial force
P
that has an eccentricity e and
is applied at a remote location from the crack. Except for the
absence of a shear force, this is similar to the loading of the
cross section of a concrete gravity dam. In this first example,
let us assume that e
=
Dl3
[Fig. l(a)).
First consider concrete to be an elastic material with zero
tensile strength. Then, the left half of the specimen carries
no stresses. This implies that the left half of the specimen is
intersected by densely distributed (continuously smeared)
cracks, as shown in Fig. l(b). In the right half, the distribution
of the axial compressive stresses is triangular [Fig. l(b)) and
the same in every horizontal cross section because the cross
sections remain plane.
In the notension design, the basic condition of safety is
that a stress distribution with no tensile stresses must exist.
If
such a distribution is found, any proportional increase of
the load will maintain the tensionfree state because the ma
terial behaves linearly in compression. So, the load capacity
is not limited by tensile behavior of the material. Instead, it
is limited by compression strength. The compression failure
of brittle materials such as concrete or rock consists of prop
agation of bands of compression splitting cracks and shear
damage bands. This failure is also brittle.
It
does not exhibit
a yield plateau. However, analysis of these phenomena is
extremely complex.
Therefore, if a stable notension state is found, the ultimate
(d)
(h)
(I)
j
.1 .1
I
.1
\
rock
joints
.1 .1 .1
IT I
.1
Yo
1. NOotoughness,2. NOotenslon, 3. NOotoughness,
\ Isolated crack Smeared cracks Close cracks
I
"V"
Dry
Joints
"
y
I open"1
~I~~ed
Principal Stress
Trajectories
RG.
1. (a) Rectangular Specimen Analyzed In Example 1; (b) Distributed Cracking Implied by NoTension design; (c,d) Stress Distributions
according to Fracture Mechanics with
K,
>
0 and
K,
=
0; (e) Approximate Trajectories of Minimum Principal Stresses for
K,
>
0; (fh)
Masonry with Dry Joints; (I) Specimen of Jointed Rock
JOURNAL OF STRUCTURAL ENGINEERING 1 JANUARY 199613
(or maximum) load
P
u
is in practice assumed to occur when
the maximum magnitude of the minimum (compressive) prin
cipal stress becomes equal to the allowable stress
crall
=
~f~,
where
f~
is a safe, low estimate of the "compression strength"
of the material and
l!~
is the safety factor, for which a rather
high value is normally assumed.
The ultimate (maximum) load
P
u
according to the elasto
plastic design, based on a zero tensile yield strength and al
lowable compression stress, is the resultant of a triangular
stress distribution [Fig. l(b)]. So,
P
u
=
~f~Dl4.
Obviously,
this is a possible solution, satisfying all the conditions of equi
librium and compatibility. But this must also be the only
possible notension solution, because the notension material
is the special limiting case of an elastoplastic material, for
which the solutions of boundary value problems (without non
linear geometric effects) are known to be unique.
Second, consider the material to have a finite tensile strength,
f:
>
O. In that case, the left half of the specimen will not
suffer continuously distributed cracking as shown in Fig. l(a).
Rather, a sharp crack will be present, as is often seen in dams.
So fracture mechanics must be used to solve the problem.
The solution can be obtained as the superposition of: (1) the
solution for centric load
P;
and (2) the solution for moment
M
=
Pe
applied on the top of the specimen. These two
solutions are available in handbooks (Tada et al. 1985; Mu
rakami 1987), according to which the mode
I
stress intensity
factor at the crack tip is
where, for a
~
0.6
FM(a)
=
1.122  1.40a
+
7.33a
2

13.08a
3
+
14.0a
4
(error
~
0.2%)
FN(a)
=
1.122  0.231a
+
1O.55a
2

21.72a
3
+
30.382a
4
(error
~
0.5%)
and, for all a
FM(a)
=
~
tan
TIa
(cos
TIa)
TIa 2 2
a
a
=
D
. [0.923
+
0.199 ( 1 
sin
TI
2
a)
4J
error
~
0.5%
FN(a)
=
~tan
TIa
(cos
TIa)1[0.752
+
2.02a
TIa 2 2
+
0.37 (1 
sin
~a)
3J
error
~
0.5%
(1)
(2)
(3)
(4)
(5)
where
N
= 
P
=
normal force in the cross sections. The
foregoing expressions apply for an infinitely long specimen
(HIL
~
00), but they are very good approximations even for
finite
H,
provided we assume
HIL
~
4. Note that
K/
char
acterizes the energy release rate
C§
because
C§
=
K7(l 
v
2
)1
E,
where
E
=
Young's modulus and
v
=
Poisson's ratio.
Substituting
N
= 
P
and
M
=
Pe
with
P
=
~f;DI4
(the
load capacity for the notension design), we now evaluate
K/
for the case a
=
aID
=
0.5 [Fig. l(a)]. The result is
K
J
=
0.0505f;V15
>
0
(6)
Now, an important point is that the stress intensity factor
K/ is positive. This means that, according to LEFM, the axial
normal stresses
cry
in the ligament of the cracked cross section
tend to +00 as the crack tip is approached [Fig. l(c)]. In
practice, of course,
cry
cannot exceed the local tensile strength
4
I
JOURNAL OF STRUCTURAL ENGINEERING
I
JANUARY 1996
of the material. But the positiveness of
K
J
has two implica
tions:
1. Tensile stresses exist within a certain portion of the hor
izontal cross section near the crack tip (in reality, of
course, these stresses are not infinite, but the resultant
of the actual tensile stresses is about the same as the
resultant of the LEFM tensile stresses at the singularity).
Consequently, for the given load
P
with eccentricity
e
=
DI3
and the given crack length
a
=
Dl2,
the design
is actually not a notension design if the finiteness of
the material tensile strength is taken into consideration.
2. Growth of the crack would cause a release of energy
from the structure. When a structure can release energy,
it does so spontaneously (according to the second law
of thermodynamics) and is unstable [Bazant and Ce
dolin (1991), Chapters 12 and 13].
As an alternative to the notension design, in which the
tensile strength of the material is also taken as zero but in a
different sense, one may propose the concept of "notough
ness" design. In this design, the critical value
K/c
of the stress
intensity factor, called the fracture toughness, is taken as zero
(i.e.,
KJc
=
0) and the stress at the crack tip cannot be un
bounded [Fig. l(d)].
If
the fracture toughness is zero, the
notension design that we obtained represents an unstable
situation. The crack will propagate dynamically. The no
toughness design is obtained for the crack length
a
for which
K
J
=
O.
From Fig. 2, we see that the curve of
K
J
versus the relative
crack length a
=
aiD
has a zero point. So the notoughness
design exists, and Newton's iterative method yields the value
a
=
0.549 (7)
Thus the stable crack is longer than that obtained by the no
tension design.
If
the crack extension from a
=
0.5 to 0.549
occurs at a constant loadpoint displacement, the load must
obviously decrease. Therefore, the loaddeflection diagram
for the notoughness design lies below that for the notension
design (Fig. 3).
In reality, the fracture toughness
KJc
is, of course, nonzero.
Then the notension design mayor might not yield a stable,
safe state. But it is important to realize that, according to
I
i
8
I
I
i
I
J

I
I
, I
 
t:,:::;;V~~
~~!!!
_
r
_s~
6
Il..
"'"
4
~
N
::;.
Q
~
2
0
,..

I
I
I
!
I
2
4
0.0
b
=
1
i
0.2
0.4
,
"
,I
, I
PN=0.4,99
I
I
r+
I
''
I ....
r , ,
,
..
~
_ ...
;~~_=~:
_____
~li",~'_~?
r 
1
~O.46:
03
~O.541J
\
I
~
N)
.4
\
I
,
I
i\
,
I
\
I
I
I I
,
I
0.6
0.8
1.0
ex
AG. 2. Dependence of Stress Intensity Factor K, on Relative Crack
Length
0:
for Various Crack Lengths a and Corresponding Eccen
tricities eN of Compression Resultant
(b)
f~
=
0
u
FIG. 3. LoadDeflection Curves for NoTension and NoTough
ness Designs
o
..
Q.
g>
Ocr
log 0
FIG. 4. Size Effect In Geometrically Similar Structures according
to Strength Criteria and Linear Elastic Fracture Mechanics
(6), the notension design will yield an unstable state for any
given value of
KIc
if the size
D
exceeds a certain value, namely
(
KIc
)2
D> 0.0505/;
(8)
This property is illustrated in Fig. 4, in which log
KJ
is plotted
versus log
D
for the plastic notension design and for LEFM.
The plots are a horizontal line and a straight line of downward
slope  112. Obviously, these two lines must intersect for a
certain size
D.
What do our results mean for rock? The notension concept
is used in geotechnical engineering because rock joints can
actually have zero tensile strength. However, the strength of
the rock between the joints [Fig. 1(g)] is usually nonzero. So,
the joints cannot be considered to be infinitely densely dis
1.0
(a)
NoTension
0.8
DeSign~
a=0.5D
p=p
u
..Q.
0.6
fd
0.4
0.2
P
0
0.6 0.8
(J' 
00
1.0
tributed, as required for the applicability of the notension
design.
If
our specimen were made of rock, the notension
design would be justified only if the spacing of the joints
(which are equivalent to cracks) were much smaller than the
crosssection dimension
D.
This is normally true for masonry
[Fig. 1(h)] but not for typical rock mechanics problems. The
value of
a
in our example represents the length of the open
portion of the joint, and the rest of the joint transmits com
pressive stresses. At the end of the open portion we must
have
K
J
=
0 because the stresses cannot be infinite. Now, if
the open portion of the joint has length
a
=
Df2,
as predicted
by the notension analysis of the joint, the resulting
K
J
value
for the end of the open portion is nonzero. The principal
stress trajectories get concentrated near the front of the open
portion of each notension joint, as approximately sketched
in Fig. 1(i). Such an opening state of the joint is unstable.
So the open portion of the joint will extend up to length
a
=
0.549D,
for which
K
J
=
O.
The situation is different when the joints of masonry have
zero strength (dry joints) and are not far apart (relative to
D),
but densely distributed. In that case, the boundary of the
compression zone of the cross section is indeed located at
approximately
a
=
Df2.
Tensile stresses between the joints
(i.e., within the bricks) exist but are very small. The tensile
principal stress trajectories are deflected by the fronts of the
open portion of the joints, but only very little, as shown by
the wavy line in Fig. 1(g).
The axial stress distributions across the uncracked liga
ment, produced by load
P
with eccentricity
e
=
D/3,
have
been obtained by the elastic finiteelement analysis, both for
ex
=
0.549 and ex
=
0.5 (Fig. 5). The stress profile for ex
=
0.5 in Fig. 5 illustrates the existence of tensile stresses near
the crack tip.
For ex
=
0.549, we see no negative stresses. The stress
profile terminates at the crack tip asymptotically as
IT
ex:
vx=a
(where coordinate
x
is the distance from the crack
mouth). This is the third term of the neartip asymptotic series
expansion (Broek 1986). The first term, proportional to
KJf
v:x=a,
vanishes because
K
J
=
O.
The second term, which
0.95
(b)
No1oughness
Design
No Tension
Design
Mechanics,
a =0.5490
P
0.8 1.0
x/D
FIG. 5. Axial Stress Distributions along Ligament of Cracked Cross Section for Load P with Eccentricity e
=
0/3
(Fig. 1) and Crack Lengths
a
=
0.50 and 0.5490
JOURNAL OF STRUCTURAL ENGINEERING
1
JANUARY
1996/5
is a constant, contributes only normal stresses parallel to the
crack.
Fig. 5 reveals that, for the same
P,
the maximum com
pressive stress magnitude in the cross section is 95% of that
for
<X
=
0.5. So, according to the allowable compressive stress
criterion, the load capacity for the notoughness design is, in
this example, 5% higher than for the notension design, even
though the loaddeflection diagram of the notoughness de
sign lies below that of the notension design (Fig. 3). So, in
this example, the notension design yields a safe estimate of
the load capacity.
This kind of conclusion, however, is not obtained in all
situations, as shown in the following example. Besides, there
is one questionable aspect: for the notoughness design, the
uncracked ligament of the cross section is smaller than for
the notension design, yet the allowable compression stress
criterion predicts the compression capacity of the ligament to
be larger. This kind of conclusion is valid only under the
hypothesis that the allowable stress is a realistic criterion for
compression failure, which is not the case.
If
the real compression failure mechanism, consisting of
propagation of splitting compression cracks or shear damage
bands, is taken into consideration, the compression failure,
too, exhibits size effect. Thus the load capacity corresponding
to compression failure must be expected to decrease with size
D.
In a manner similar to that in Fig. 4, for tensile failure,
if a certain size is exceeded, the actual load capacity could
become lower than the load capacity for notension analysis
with allowable compression stress, which is known to exhibit
no size effect.
The foregoing conclusion concerns only the overload by
axial load
P.
If,
subsequent to load
P
causing the crack to
extend up to length
a
=
0.549D, a horizontal shear force P
x
is superimposed as an additional load, the shear capacity of
the specimen will be lower than that predicted by the no
tension design for the crack of length
a
=
0.5D. The reason
is that the length of the un cracked ligament, D  a
=
0.451D
[which is available to resist sliding due to shear loading; WES
(1983)], is smaller than for the notension design, for which
D  a
=
0.5D. This conclusion is important for the earth
quake loading of dams.
EXAMPLE 2: REMOTE APPLIED FORCE AND CRACK
FACE PRESSURE
Let us now consider the same specimen with relative crack
length
<X
=
0.5, but with a different loading. In addition to
the remotely applied axial force
P,
the crack faces (all the
way to the crack tip) are loaded by uniform pressure
p
due
to water that penetrates the crack. Such loading occurs in
cracked dams. Let us assume that
P
and
p
grow proportion
ally, setting
p
=
pPID where p is a given coefficient. For a
typical dam profile, p
=
0.6 at full reservoir. We will assume
the value of
p
to be precisely p
=
0.6153 (this number has
been chosen simply because the finiteelement results were
already available for this value). The eccentricity of load
P
(Fig. 6) is assumed to be precisely e
=
0.1539D [this is a
value for which the loads applied on the upper half of the
specimen above the cracked cross section in Fig. 6(a) are in
balance with a triangular stress profile through the ligament,
i.e., the uncracked part of the cross section].
First, consider notension plastic limit analysis. The frac
ture front cannot remain sharp, or else singular stresses tend
ing to
+
00,
which violate any strength limit, would develop
and the notension analysis would thus predict the crack to
run all the way across the ligament, for any positive load
P,
no matter how small. So, the crack front must widen. Thus,
despite pressure
p
on the crack faces, smeared (densely dis
tributed) cracks must develop parallel to the crack faces [Fig.
6/ JOURNAL OF STRUCTURAL ENGINEERING / JANUARY 1996
6( c)]. This is possible if we consider the tensile strength to
be zero and assume that water of pressure
p
permeates also
these parallel cracks.
The notension solution is easily found if the entire left half
of the specimen is assumed to undergo smeared horizontal
cracking. Then each horizontal cross section is in the same
stress state and remains plane. Thus, the stress distribution
across the right half of the cross section is triangular, as shown
in Fig. 6(c) (at the limit state of notension design, the stress
profile must have a jump from 
p
to 0 at the cracking front).
The vertical condition of equilibrium of the top half of the
specimen yields P  pPI2
=
IJf; Dl4, and so the ultimate
load is
p
=
P"
=
0.3611lJf;D
(9)
Admittedly, the aforementioned process of spreading of
pressurized cracks according to the zero tensile hypothesis
involves conceptual difficulties. But example 2 is not irrele
vant for current practice because notension finiteelement
calculations for dams with pressurized cracks have been car
ried out. In the discrete form (finiteelement analysis), the
conceptual difficulties we alluded to do not arise. But they
cannot really be completely ignored because refinement of
the element size to zero must yield the continuum solution.
Second, consider that the material tensile strength is not
zero but finite, and the crack extension is governed by the
LEFM fracture toughness criterion (which is equivalent to
the energy release criterion). The finiteness of strength im
plies that the strip of width al2 (left half of the specimen)
cannot be cracked in a continuous, smeared manner. When
a crack forms, other cracks cannot form near it because the
stress in the material on the sides of the crack is reduced. So,
stress concentrations at the crack tip must arise and fracture
mechanics must be used.
By virtue of the linearity of LEFM, the solution can be
obtained by superposing the solutions of the two loading cases
shown in Fig. 6(b): Case A, in which uniform pressure
p
is
applied on top of an uncracked specimen; and case B, in
which uniform tension
p
over the entire top and concentrated
force
P
of eccentricity
e
are applied on the cracked specimen.
The values of
K[
for these two cases are superimposed. For
case A, a state of homogeneous compression
a
= 
p
is
obtained, and so
Kr
=
O. Nonzero
Kr
can be produced only
in case B, which is again solved by (2)(5). The axial force
resultant and the bending moment to be substituted in these
equations are
N
=
pD  P
=
(p  1)P (taken negative if
compressive) and
M
=
Pe.
For a crack of length a
=
0.5D and the given loading with
P
=
P
u
=
0.6499IJf;D, (2)(5) again yield a positive
Kr
value. So the crack that we found to be stable according to
the notension design is again found to be unstable according
to fracture mechanics and to propagate dynamically. (Even
if the fracture toughness
KIc
were finite, the nopropagation
criterion
Kr :::; K/c
would always be violated for a sufficiently
large
D,
as before.)
The next question is whether a stable crack with
K,
=
0
exists for 0.5D
<
a
<
D. For the given load P of eccentricity
e
=
0.1539D and uniform crack face pressure
p
=
pPID
=
0.6153PID extending up to the tip, we can calculate from (2)
(5) the curve of
K,
as a function of
<X.
To this end, we sub
stitute the
M
and
N
values for the loading case B, that is,
moment
M
=
Pe and centric force
N
=
pD  P
=
(p 
1)P (where
N
is taken as negative if compressive). This is
equivalent to loading by axial force
N
with eccentricity eN
=
 MIN
=
el(1  p)
=
0.1539D1(1  0.6153)
=
0.4000D.
The calculated curve of K[ is shown in Fig. 2 for eNID
=
0.4.
We see the curve has a zero point. This means that a stable
(al
(b)
p


+
A
p
r
1
N
!
I
II
B
(c)
p
p
FIG. 6. (a) Rectangular Specimen with Crack Face Pressure p Analyzed In Example 2; (b) Equivalent Superposition of Loading Cases A
and B; (c) Stress Distribution In Case of Pressurized Densely Distributed Cracks
crack does exist for the given loading. Iterative solution of
the root shows that
K{
=
0 occurs precisely for
0:
=
0.725
(10)
For this crack length and for zero toughness (K{c
=
0), the
loads
P
and
p
that the specimen can carry are limited only
by the capacity of the material to resist compression, which
may be approximately characterized in terms of the allowable
compression stress
JJ.J;.
The stress distribution across the un
cracked ligament, which has been calculated by finite ele
ments, is plotted in Fig. 7(b), in which the maximum com
pressive stress magnitude is<T
=
3.25PID.
Setting this equal
to
JJ.J;,
we get
(11)
This represents 85% of the ultimate load capacity
P
u
pre
dicted by the notension approach. So we have an example
aD
P
aD
p
(a)
2
D/P=0.615
0'=0
0
alo.500,,"
0 0.2 0.4 0.6 0.8 1.0
3
(b)
2
K
J
=0
810.725~
ooL~0~.2~0.40~.6~~0~.8~1.0
x/D
FIG. 7. Stress Distributions in Cracked Cross Section of Speci
men with Crack Face Pressure (Example 2) for: (a) NoTension
Design; (b) NoToughness Design
that the notension design not only can yield an unstable
crack, but also can significantly overpredict the load capacity
of the structure.
Similar results can be obtained for other crack lengths. This
is clear from the curves of
K{
versus ex shown in Fig. 2 for
various increasing values of
eN
corresponding to increasing
values of
a.
As
a
~
D
(which corresponds to
eN
~
D12) ,
these curves approach at
x
=
DI2
a dipole, that is a jump
from
+
00
to 
00.
The crack length
a
<
DI2
for which
K{
=
o
always exists and approaches
a
~
D.
As
pDIP
approaches
0.6922, both
a
o
for the notension design and
a
for the no
toughness design approach
1.
For
pDIP
>
1 
(2e/D)
=
0.6922, both the notension and notoughness designs cease
to exist.
It might seem strange that for
K{
=
0 the stress profile in
Fig. 7(b) does not have a zero stress at the crack tip even
though crack propagation is incipient. To understand that this
must be so, observe two facts: (1) For a crack of length
a
=
0.725D(1
+
8) (where 8 is arbitrarily small), the Krvalue
would be positive, and thus LEFM would give an infinite
tensile stress ahead of the tip [Fig. 8(a»), the physical meaning
of which is that the energy release rate is nonzero; and (2)
for a crack of length
a
=
0.725D(1 
8), the Krvalue would
be negative, and thus LEFM would give an infinite com
pressive stress ahead of the tip [Fig. 8(c»), which would be
impossible because it would imply an overlap of the crack
faces. So, as
a
grows, the LEFM stress must jump from
+
00
to
00
at
0:
=
0.725. The difference from the critical stress
profile for the notension limit design [Fig. 7(a») illustrates
Griffith's fundamental idea: the propagation of a sharp crack
FIG. 8. Stress Distributions in Cracked Cross Section of Speci
men with Crack Face Pressure (Example 2) for Various Values of
Stress Intensity Factor K,
JOURNAL OF STRUCTURAL ENGINEERING / JANUARY 1996/7
must be decided by the critical energy release rate (or fracture
toughness) rather than the material strength.
The loading with crack face pressure has the particular
feature that, because of the difference in crack length, the
ratio of the pressure resultant pa to the axial load
P
is not
the same for the notension and notoughness designs when
the ratio of
p
to
D
is the same. Whether, for a loading without
crack face pressure, the load capacity according to fracture
mechanics could be less than the load capacity according to
the notension design is not known at present. This question
should be researched further.
ANALYSIS OF PRESENT RESULTS
Both examples demonstrate that the crack length obtained
from the notension plastic design can be unstable if the fi
niteness of the material strength is taken into account. For
zero fracture toughness, the crack is unstable in these ex
amples for any size
D,
while for finite fracture toughness it
becomes unstable only when a certain size
D
is exceeded.
Example 2, as well as example 1 with horizontal load P
x
superimposed after crack formation, further demonstrates that
the load capacity obtained by fracture mechanics can be less
than that obtained by the notension design. This is true not
only for the notoughness design, but also, for a large enough
structure, for a design with finite fracture toughness. As men
tioned, this conclusion may be understood on observing that
a structure of a nonzero tensile strength can store more energy
than a structure of zero tensile strength, and can thus release
energy during crack propagation at a higher rate.
Another simple, albeit partial, explanation is provided by
the size effect. The plastic notension design exhibits no size
effect, while failures controlled by fracture mechanics exhibit
a size effect such that the nominal strength for similar failures
of geometrically similar structures of different sizes decreases
in inverse proportion to the structure size
D,
as illustrated in
Fig. 4. From this it follows that if the cracks are geometrically
similar, there must exist a structure size
Dcr
for which the
nominal strength of the structure becomes less than the strength
obtained by the notension plasticity. However, this expla
nation does not apply if
K[
=
0 and if the load capacity is
assumed to be controlled by the allowable compressive stress,
for which there is no size effect.
The zero tensile strength assumption is nevertheless correct
if the cracks are known to be densely distributed. In other
words, the assumption is correct if the cracks do not localize.
Aside from the case of dry joint masonry mentioned, this is
the case for bending cracks in a reinforcedconcrete beam,
provided the reinforcement ratio exceeds a certain minimum
value [Bazant and Cedolin (1991), Chapter 12].
The problem with the notension design may be intuitively
understood from the shape of the principal stress trajectories,
which are sketched for the case of cracked specimens with
finite and zero tensile strengths in Fig. 1( e,f). The trajectories
of the tensile and compressive principal stresses are shown
by the solid and dashed lines. The tensile stress field develops
high stress concentrations at places where the adjacent prin
cipal stress trajectories approach each other. The solid curves
in Fig. l(e), representing the tensile principal stress trajec
tories, are deflected by the crack tip because they must pass
around it. This forces the trajectories to become very close
to each other in the vicinity of the crack tip. By contrast, in
the case of notension design, which corresponds to the con
tinuously distributed cracking in the left half of the specimen
in Fig. l(b), all the principal stress trajectories are parallel
vertical lines. The tensile response at zero tensile strength is
of a plastic nature. Plasticity blunts a crack, forcing the crack
ing front to be smooth.
The present results further reveal an amazing effect: an
8 I
JOURNAL OF STRUCTURAL ENGINEERING
I
JANUARY 1996
increase in the tensile strength of the material can cause a
reduction of the load capacity of the structure, with all other
geometric and material characteristics being the same. In plas
ticity, this effect is impossible.
The basic conclusion from the present examples, as well
as some recent finiteelement studies (to be reviewed), is that
the notension limit design of concrete or rock structures
cannot guarantee that the actual safety factor will have the
value specified by the building code. The notension design
will nevertheless remain a useful tool, because of its simplic
ity. The classical applications of this design approach to dams
or tunnels have no doubt been safe, especially in view of the
large values of the safety factors used in design.
The present study nevertheless demonstrates that if the
design is not based on fracture mechanics, it should at least
be checked by fracture mechanics. Designing on the basis of
fracture mechanics would make it possible to achieve more
uniform safety margins and, thus, either permit a lowering
of the safety factors or a further decrease in the already ex
tremely small probabilities of failure.
ANALYSIS OF PREVIOUS FINITEELEMENT RESULTS
Most of the present observations have in essence already
been made in the studies by Bazant (1990) and Gioia et at.
(1992), although not on the basis of such simple examples.
The Gioia et at. study involved finiteelement calculations,
which will be reviewed briefly, for the sake of completeness
of the arguments.
A cracked specimen of finite length
L
was considered sub
jected to a combination of axial load
P
and bending moment
M, which resembles the loading of a dam (Fig. 9). Using
fracture mechanics solutions from handbooks and assuming
that
K[
=
1, Bazant (1990) calculated the eccentricity e of
the compression resultant in the uncracked ligament of the
cracked cross section. Various values of the relative crack
length aiD were considered. The distance of the compression
resultant from the right side of the specimen is
(DI2) 
e,
while according to the plastic notension design, for which
the stress distribution in the ligament is triangular, this dis
tance is
(D  a)/3.
Thus, the ratio
(DI2) 
e
P
=
(D  a)/3
(12)
characterizes the change of the location of the compression
resultant compared to the plastic notension design. In the
case of a dam, the closer the compression resultant toward
the end of the ligament, the lower the safety of the structure.
r
d d
'2"
"2"
H
M
1
~
p
l!JJJ
'2" ' '2"
I
FIG. 9. Example Analyzed In Baiant (1990) and Location of
Compression Resultant and Stress Distribution for K,
=
0
2
,
o
o
(d/2)e
, (dU/3
0.2
r1.25
0.4
0.6
0.8
Q
FIG. 10. Ratio p of Distances of Compression Resultant from End
of Ligament Calculated In Bmnt (1990) for NoToughness and No
Tension Designs (Values p
<
1 Indicate Cases where NoTension
Design Gives Unsafe Estimate of Resultant Location)
Thus, the values p
~
1 indicate the cases for which the plastic
notension design yields the safe location of the compression
resultant, and the values p
<
1 indicate the cases for which
the plastic notension design yields an unsafe location. The
values of the ratio p as a function of the relative crack length
are plotted in Fig. 10 for various values of the ratio
r 
HI
D,
where
H
=
height of the specimen [for a table of the
0.75 MPa
~
....
t
0.25 MPa.="r........
+........ "'"
0.25 MPa
~~~~"""'J
AddftlonaJ Overflow
(b)
FulR888fV'01r
I'nIIIauI8
l
values of p, see Bazant (1990)]. There are many cases in which
p
<
1.
A finiteelement study of the safety of the notension design
of dams was undertaken by Gioia et al. (1992). The geometry
of the cross section of the Koyna dam (Saouma et al. 1990),
which was stricken by an earthquake in 1967, was considered
[Fig. l1(c) shows the finiteelement mesh and the shape of
the critical crack for the loading considered]. Finiteelement
solutions according to notension plasticity and according to
fracture mechanics were compared [Fig. l1(c,d)]. The yield
surface for notension plasticity [Fig. l1(a)] was a special case
of Ottosen's (1977) yield surface for the tensile yield strength
approaching zero. Because the origin of the stress space must
lie inside the yield surface, the calculations have actually been
run for a very small but nonzero value of the tensile yield
strength of concrete, approximately 10 times smaller than a
realistic value. Similarly, the notoughness design was ap
proximated in the finiteelement calculations by taking the
K/cvalue to be approximately 10 times smaller than the re
alistic value. The crack length obtained by fracture mechanics
is, in this problem, very insensitive to the
Krcvalue
because
Kr
represents a small difference of two large values
Kr
due
to water pressure minus
Kr
due to gravity load.
Similar to the present two examples, the differences be
tween notension limit design and fracture mechanics have
been found to be the most pronounced for the case when
water penetrates into the crack and applies pressure on the
crack faces. Because plastic analysis cannot describe crack
propagation, the dam has been assumed to be precracked and
loaded by water pressure along the entire crack length.
In the calculations, some of whose results are plotted in
Fig. 11( c,d), the height of the water overflow above the crest
of the dam was considered as the load parameter. A down
ward curving crack, which was indicated by calculations to
be the most dangerous crack, was considered. From the re
sults in Fig. 11 (c), it is seen that the diagram of the load
parameter, taken as the overflow height, versus the horizontal
displacement at the top of the dam lies lower for fracture
mechanics than it does for notension plasticity. In other words,
the resistance offered by the dam to the loading by water is
(c)
~10
S
:t
~6
~
Fracture. K
1C
=
0
2
Full crack pressure
0.02 0.04 0.06 0.08
Displacement at Top (m)
5
(d)
:§:
~
3
'E
CD
c3
Fracture Mechanics
Realf;. K
1c
0.02 0.04 0.06 0.08
Displacement at Top (m)
FIG. 11. Koyna Dam Analyzed In Gioia et al. (1992): (a) Yield Surfaces of Concrete; (b) FiniteElement Mesh and Failure Mode; (c)
Comparison of Curves of OverflOW Height versus Deflection for NoTension Limit Analysis and NoToughness Fracture Analysis; (d) Curves
for Limit Analysis and Fracture Analysis with Realistic Values of Strength and Toughness
JOURNAL OF STRUCTURAL ENGINEERING
1
JANUARY
1996/9
lower according to the fracture mechanics solution, with a
realistic value of the fracture toughness
KIn
than it is ac
cording to notension plasticity. Fig. l1(c,d) shows some typ
ical calculated diagrams of load parameter versus displace
ment at the top of the dam for realistic values of the fracture
toughness and the tensile yield strength
t; .
It
should be added
that, for these finiteelement calculations, the maximum of
the loaddeflection diagram could not be reached for realistic
heights of overtopping of the dam. This is because the down
ward curvature of the critical crack tends to prevent the static
loaddeflection curve from flattening out. Thus, comparisons
of the static load capacities were not possible for the geometry
of the Koyna dam.
CONCLUSIONS
1.
For a brittle (or quasibrittle) elastic structure, the elas
ticperfectly plastic analysis with a zero value of the
tensile yield strength of the material is not guaranteed
to be safe because it can happen that:
The calculated length of cracks or cracking zones cor
responds to an unstable state of crack propagation
The uncracked ligament of the cross section, available
for resisting horizontal sliding due to shear loads, is
predicted much too large, compared to the fracture
mechanics prediction
The calculated loaddeflection diagram lies lower than
that predicted by fracture mechanics
The load capacity for a combination of crack face pres
sure and loads remote from the crack front is predicted
much too large, compared to the fracture mechanics
prediction.
2. Due to the size effect, the preceding conclusions are
true not only for zero fracture toughness (notoughness
design), but also for finite fracture toughness, provided
the structure is large enough.
3. The notension limit design cannot always guarantee the
safety factor of the structure to have the specified value.
Fracture mechanics is required for that.
4. Increasing the tensile strength of the material can cause
the load capacity of a brittle (or quasibrittle) structure
to decrease or even drop to zero.
5. The notension limit design would be correct if the ten
sile strength of the material were actually zero through
out the structure. This is true for dry masonry with
sufficiently densely distributed joints, but not for con
crete or for jointed rock masses.
6. The finiteness of the tensile strength of the material at
points farther away from the cracks or rock joints (or
construction joints) of negligible tensile strength causes
the structure to store more strain energy. Thus, energy
can be released during fracture propagation at a higher
rate. This is one simple explanation of the present find
ings. Another simple explanation is the fact that a sharp
crack tip causes stress concentrations, as manifested by
crowding of the principal stress trajectories near the
crack tip. When the material tensile strength is zero
throughout the structure, the behavior is plastic in ten
sion; this causes the cracking front to be smooth and
thus prevents stress concentrations. Still another expla
nation (although only a partial one because it does not
apply to failures controlled by allowable compressive
stress) is the fact that failures controlled by strength
criteria, even for zero tensile strength, exhibit no size
effect whereas failures controlled by fracture mechan
ics do.
10
I
JOURNAL OF STRUCTURAL ENGINEERING
I
JANUARY 1996
ACKNOWLEDGMENTS
Partial financial support under NSF Grant No. BCS8818230 to North
western University is gratefully acknowledged. Thanks are due do Yuan
Neng Li, Research Assistant Professor, and Zhengzhi Li, Graduate Re
search Assistant, for their help in some of the computations.
APPENDIX. REFERENCES
Bazant, Z. P. (1984). "Size effect in blunt fracture: rock, concrete,
meta!."
J.
Engrg. Mech.,
ASCE, 110(4),518535.
Bazant, Z. P. (1990). "A critical appraisal of 'notension' dam design:
a fracture mechanics viewpoint."
Dam Engrg.,
1(4),237247.
Bazant, Z. P. (1990). "Errata of 'a critical appraisal of "notension"
dam design: a fracture mechanics viewpoint. '"
Dam Engrg., 2(2).
Bazant, Z. P. (1994). "Recent advances in fracture mechanics, size effect
and rate dependence of concrete: implication for dams."
Proc., Int.
Workshop on Dam Fracture and Damage,
A. A. Balkema, Rotterdam,
The Netherlands, 4154.
Bazant, Z. P., and Cedolin,
L.
(1991).
Stability of structures: elastic,
inelastic, fracture and damage theories.
Oxford University Press, New
York, N.Y.
Bazant, Z. P., and Kazemi, M.
T.
(1990). "Size effect in fracture of
ceramics and its use to determine fracture energy and effective process
zone length."
J.
Am. Ceramic Soc.,
73(7), 18411853.
Bazant, Z. P., He, S., Plesha, M. E., and Rowlands, R. E. (1991).
"Rate and size effect in concrete fracture: implications for dams."
Proc., Int. Conf. on Dam Fracture;
Pub!. 957491, V. Saouma, R.
Dungar, and D. Morris, eds., Electric Power Res. Inst., Palo Alto,
Calif., 413425.
Bourdarot, E., Mazars, J., and Saouma, V. E. (eds.). (1994). "Dam
fracture and damage."
Proc. Int. Workshop on Dam Fracture and
Damage,
A. A. Balkema, Rotterdam, The Netherlands.
Broek, D. (1986).
Elementary engineering fracture mechanics,
4th Ed.,
Martinus Nijhoff Publishers, Dordrecht, The Netherlands.
Brown, W. F., and Srawley, J. E. (1967). "Fracture toughness testing
methods."
Fracture toughness testing and its applications; STP 381,
ASTM, Philadelphia, Pa.
Bureau of Reclamation (BuRec). (1987).
Design of small dams,
U.S.
Dept. of the Interior, Denver, Colo.
Dungar, R., Saouma, V. E., and Wittmann, F. H. (eds.). (1990).
Work
shop notes: research workshop on "Application of fracture mechanics
to dam engineering."
Swiss Federal Inst. of Techno!. (ETH), Ziirich,
Switzerland.
Gioia, G., Bazant, Z. P., and Pohl, B. (1992). "Is notension dam design
always safe?"
Dam Engrg.,
3(1), 2334.
Gioia, G., Bazant, Z. P., and Pohl, B. (1992). "Closure to 'Is notension
dam design always safe?'"
Dam Engrg.,
4(1), 59.
Gross, B., and Srawley, J. E. (1964). "Stress intensity factors for a single
edgenotch tension specimen by boundary collocation of a stress func
tion."
Rep. NASA TN D2395.
He, S., Plesha, M. E., Rowlands, R. E., and Bazant, Z. P. (1992).
"Fracture energy tests of dam concrete with rate and size effects."
Dam Engrg.,
3(2), 139159.
Hodge, P. G. (1959).
Plastic analysis of structures,
McGrawHill Book
Co., Inc., New York, N.Y.
Jansen, R. B. (1988). "Advanced dam engineering for design, construc
tion and rehabilitation." Rep., U.S. Dept. of Interior, Denver, Colo.
Murakami, Y. (ed.) (1987).
Stress intensity factors handbook; Vol. I,
Pergamon Press, Oxford, England.
Ottosen, N. S. (1977). "A failure criterion for concrete."
J.
Engrg.
Mech.,
ASCE, 103(4), 527535.
Owen, D. R. J., and Hinton, E. (1980).
Finite elements in plasticity,
Pine ridge Press, Swansea, Wales.
Saouma, V. E., Dungar, R., and Morris, D. (eds.). (1991). "Dam frac
ture."
Proc., Int. Conf. on Dam Fracture; Publ. GS7491,
Electric
Power Res. Inst., Palo Alto, Calif.
Saouma, V. E., Briihwiler, E., and Boggs, H.
L.
(1990). "A review of
fracture mechanics applied to concrete dams."
Dam Engrg.,
1 (1),
4158.
Tada, H., Paris, P. C., and Irwin,
J.
K. (1985).
The stress analysis of
cracks handbook,
2nd Ed., Paris Productions, Inc., St. Louis, Mo.
Tardieu, B., and Londe, P. (1992). "Discussion of Bazant, Gioia and
Pohl (1992)."
Dam Engrg.,
3(4), 301.
Waterways Experiment Station (WES). (1983). "Design of gravity dams
on rock foundations: sliding stability assessment by limit equilibrium
and selection of shear strength parameters."
Tech. Rep. GL83J3,
U.S. Army Corps of Engrs., Vicksburg, Miss.
Zienkiewicz, O.
C.
(1971).
The finite element method in engineering
science,
McGrawHill Book Co., Inc., London, England.
Σχόλια 0
Συνδεθείτε για να κοινοποιήσετε σχόλιο